See all Blog Posts Welding Cast Iron: Tips to Avoid Cracking Category: Processes Posted: June 14, 2022 Welding cast iron is known to be notoriously difficult. Does this hold true for all types of cast iron? And what about it makes it so difficult to weld? In this article, we explore the unique crystallography and welding of ductile and gray cast iron, detailing the techniques you can use to get the job done right. For the purposes of this conversation, white cast iron is being omitted, since it is unweldable. Ductility of cast iron The difficulties with welding cast iron stem from one major issue – it’s extremely brittle. Cast iron is an iron alloy which contains more than 2.11% carbon (whereas steels contain less than 2.11%); a higher concentration of carbon content reduces ductility in metals. The carbon content in cast iron generally ranges from 2 to 4 percent. By comparison, the carbon percentage in Steel and Alloy Steel differ depending on the grade. Low-carbon steel is characterized by a low ratio of carbon to iron, consisting of less than 0.3% carbon – the ever popular mild steel 1018 steel, which has about 0.14 to 0.2 percent carbon content, falls into this spectrum. Medium-carbon steel has a higher ratio of carbon to iron, medium-carbon steel contains anywhere from 0.3% to 0.6% carbon. High-carbon steel has the highest ratio of carbon to iron, known as carbon tool steel, with around 0.61% to 1.5% carbon. Why does this carbon content matter? When an area of cast iron is heated, the carbon from surrounding areas migrates to the heated area. This further increases the carbon content and the brittleness of the area. The higher the carbon content, the more likely that the cast iron forms martensite as it cools, one of the hardest and most brittle allotropes of iron. Heating and cooling Brittleness only comes into play when there are stresses on the material. When cast iron is heated and cooled quickly and unevenly, it tends to shatter, unlike low carbon steels which simply deform and stretch the stresses away. The resulting martensite creates a strained body centered tetragonal crystal form which contains many crystal dislocations, a source of both strength and brittleness. As the heated cast iron cools, it shrinks. While it has a similar coefficient of thermal expansion to that of steels, because of its low ductility, the crystal structure doesn’t reorganize itself to smooth out the stresses. Instead, it tends to break and snap at the point(s) where there is great stress. This typically happens along the weld joints. Tips for welding cast iron Clean the cast iron before welding. Remove any impurities on the surface of the metal, paying close attention to the welding area. Preheat the workpiece. By heating and cooling your workpiece evenly, it is less likely to gain stresses and crack. Avoid long localized exposures to high heat. Move the workpiece around and make small welds at a time. Cool your workpiece slowly, in an oven. Cooling it in the air will reduce the temperature of the outside surface faster than the inside, introducing strain on the workpiece. Metal Supermarkets Metal Supermarkets is the world’s largest small-quantity metal supplier with over 100 brick-and-mortar stores across the US, Canada, and United Kingdom. We are metal experts and have been providing quality customer service and products since 1985. At Metal Supermarkets, we supply a wide range of metals for a variety of applications. Our stock includes: mild steel, stainless steel, aluminum, tool steel, alloy steel, brass, bronze and copper. We stock a wide range of shapes including: bars, tubes, sheets, plates and more. And we can cut metal to your exact specifications. Visit one of our 100+ locations across North America today. Share: Facebook Twitter LinkedIn E-Mail Tags: cast iron, welding, welding cast iron Related blog articles Local Entrepreneur Brings Metal Supermarkets to Austin, Texas What Are The Types of Metal Fabrication? Proteus: The World’s First Uncuttable Metal?